Organic electronics
Organic electronics is a field of materials science concerning the design, synthesis, characterization, and application of organic molecules or polymers that show desirable electronic properties such as conductivity. Unlike conventional inorganic conductors and semiconductors, organic electronic materials are constructed from organic (carbon-based) molecules or polymers using synthetic strategies developed in the context of organic chemistry and polymer chemistry. One of the promised benefits of organic electronics is their potential low cost compared to traditional electronics. Attractive properties of polymeric conductors include their electrical conductivity (which can be varied by the concentrations of dopants) and comparatively high mechanical  flexibility. Challenges to the implementation of organic electronic materials are their inferior thermal stability, high cost, and diverse fabrication issues. Traditional conductive materials are inorganic, especially metals such as copper and aluminum as well as many alloys. History. In 1862 Henry Letheby described polyaniline, which was subsequently shown to be electrically conductive. Work on other polymeric organic materials began in earnest in the 1960s. For example in 1963, a derivative of tetraiodopyrrole was shown to exhibit conductivity of 1 S/cm (S = Siemens). In 1977, it was discovered that oxidation enhanced the conductivity of polyacetylene. The 2000 Nobel Prize  in Chemistry was awarded to Alan J. Heeger, Alan G. MacDiarmid, and Hideki Shirakawa jointly for their work on polyacetylene and related conductive polymers. Many families of electrically conducting polymers have been identified including polythiophene, polyphenylene sulfide, and others. J.E. Lilienfeld first proposed the field-effect transistor in 1930, but the first OFET was not reported until 1987, when Koezuka et al. constructed one using Polythiophene which shows extremely high conductivity. Other conductive polymers have been shown to act as semiconductors, and newly synthesized and characterized compounds are reported weekly in prominent research journals. Many review articles exist documenting the  development of these materials. In 1987, the first organic diode was produced at Eastman Kodak by Ching W. Tang and Steven Van Slyke. In the 1950s, organic molecules were shown to exhibit electrical conductivity. Specifically, the organic compound pyrene was shown to form semiconducting charge-transfer complex salts with halogens. In 1972, researchers found metallic conductivity (conductivity comparable to a metal) in the charge-transfer complex TTF-TCNQ. André Bernanose was the first person to observe electroluminescence in organic materials, and Ching W. Tang, reported fabrication of an OLED device in 1987. The OLED device incorporated a double-layer structure  motif composed of copper phthalocyanine and a derivative of perylenetetracarboxylic dianhydride. In 1990, a polymer light emitting diodes was demonstrated by Bradley, Burroughes, Friend. Moving from molecular to macromolecular materials solved the problems previously encountered with the long-term stability of the organic films and enabled high-quality films to be easily made. In the late 1990's, highly efficient electroluminescent dopants were shown to dramatically increase the light-emitting efficiency of OLEDs These results suggested that electroluminescent materials could displace traditional hot-filament lighting. Subsequent research developed multilayer polymers and the new field of plastic electronics and organic light -emitting diodes (OLED) research and device production grew rapidly. Conductive organic materials. Organic conductive materials can be grouped into two main classes: polymers and conductive molecular solids and salts. Polycyclic aromatic compounds such as pentacene and rubrene often form semiconducting materials when partially oxidized. Conductive polymers are often typically intrinsically conductive or at least semiconductors. They sometimes show mechanical properties comparable to those of conventional organic polymers. Both organic synthesis and advanced dispersion techniques can be used to tune the electrical properties of conductive polymers, unlike typical inorganic conductors. Well-studied class of conductive polymers include polyacetylene, polypyrrole, polythiophenes, and  polyaniline. Poly(p-phenylene vinylene) and its derivatives are electroluminescent semiconducting polymers. Poly(3-alkythiophenes) have been incorporated into prototypes of solar cells and transistors. Organic light-emitting diode. An OLED (organic light-emitting diode) consists of a thin film of organic material that emits light under stimulation by an electric current. A typical OLED consists of an anode, a cathode, OLED organic material and a conductive layer. OLED organic materials can be divided into two major families: small-molecule-based and polymer-based. Small molecule OLEDs (SM-OLEDs) include tris(8-hydroxyquinolinato)aluminium fluorescent and phosphorescent dyes, and conjugated dendrimers. Fluorescent dyes can  be selected according to the desired range of emission wavelengths; compounds like perylene and rubrene are often used. Devices based on small molecules are usually fabricated by thermal evaporation under vacuum. While this method enables the formation of well-controlled homogeneous film; is hampered by high cost and limited scalability. Organic field-effect transistor. An Organic field-effect transistor is a field-effect transistor utilizing organic molecules or polymers as the active semiconducting layer. A field-effect transistor (FET) is any semiconductor material that utilizes electric field to control the shape of a channel of one type of charge carrier , thereby changing its conductivity. Two major classes of FET are n-type and p-type semiconductor, classified according to the charge type carried. In the case of organic FETs (OFETs), p-type OFET compounds are generally more stable than n-type due to the susceptibility of the latter to oxidative damage. As for OLEDs, some OFETs are molecular and some are polymer-based system. Rubrene-based OFETs show high carrier mobility of 20–40 cm/(V·s). Another popular OFET material is Pentacene. Due to its low solubility in most organic solvents, it's difficult to fabricate thin film transistors (TFTs) from pentacene  itself using conventional spin-cast or, dip coating methods, but this obstacle can be overcome by using the derivative TIPS-pentacene. Organic electronic devices. Organic solar cells could cut the cost of solar power compared with conventional solar-cell manufacturing. Silicon thin-film solar cells on flexible substrates allow a significant cost reduction of large-area photovoltaics for several reasons: Inexpensive polymeric substrates like polyethylene terephthalate (PET) or polycarbonate (PC) have the potential for further cost reduction in photovoltaics. Protomorphous solar cells prove to be a promising concept for efficient and low-cost photovoltaics on cheap and flexible substrates for  large-area production as well as small and mobile applications. One advantage of printed electronics is that different electrical and electronic components can be printed on top of each other, saving space and increasing reliability and sometimes they are all transparent. One ink must not damage another, and low temperature annealing is vital if low-cost flexible materials such as paper and plastic film are to be used. There is much sophisticated engineering and chemistry involved here, with iTi, Pixdro, Asahi Kasei, Merck & Co.|Merck, BASF, HC Starck, Hitachi Chemical and Frontier Carbon Corporation among the leaders. Electronic devices based on  organic compounds are now widely used, with many new products under development. Sony reported the first full-color, video-rate, flexible, plastic display made purely of organic materials; television screen based on OLED materials; biodegradable electronics based on organic compound and low-cost organic solar cell are also available. Fabrication methods. Small molecule semiconductors are often insoluble, necessitating deposition via vacuum sublimation. Devices based on conductive polymers can be prepared by solution processing methods. Both solution processing and vacuum based methods produce amorphous and polycrystalline films with variable degree of disorder. "Wet" coating techniques require polymers to be dissolved in  a volatile solvent, filtered and deposited onto a substrate. Common examples of solvent-based coating techniques include drop casting, spin-coating, doctor-blading, inkjet printing and screen printing. Spin-coating is a widely used technique for small area thin film production. It may result in a high degree of material loss. The doctor-blade technique results in a minimal material loss and was primarily developed for large area thin film production. Vacuum based thermal deposition of small molecules requires evaporation of molecules from a hot source. The molecules are then transported through vacuum onto a substrate. The process of condensing  these molecules on the substrate surface results in thin film formation. Wet coating techniques can in some cases be applied to small molecules depending on their solubility. Organic solar cells. Organic semiconductor diodes convert light into electricity. Figure to the right shows five commonly used organic photovoltaic materials. Electrons in these organic molecules can be delocalized in a delocalized π orbital with a corresponding π* antibonding orbital. The difference in energy between the π orbital, or highest occupied molecular orbital (HOMO), and π* orbital, or lowest unoccupied molecular orbital (LUMO) is called the band gap of organic photovoltaic materials. Typically , the band gap lies in the range of 1-4eV. The difference in the band gap of organic photovoltaic materials leads to different chemical structures and forms of organic solar cells. Different forms of solar cells includes single-layer organic photovoltaic cells, bilayer organic photovoltaic cells and heterojunction photovoltaic cells. However, all three of these types of solar cells share the approach of sandwiching the organic electronic layer between two metallic conductors, typically indium tin oxide. Organic field-effect transistors. An organic field-effect transistor consists of three major components: the source, the drain and the gate. Generally, a field -effect transistor has two plates, source in contact with drain and the gate respectively, working as conducting channel. The electrons move from source to the drain, and the gate serves to control the electrons' movement from source to drain. Different types of FETs are designed based on carrier properties. Thin film transistor (TFT), among them, is an easy fabricating one. In a thin film transistor, the source and drain are made by directly depositing a thin layer of semiconductor followed by a thin film of insulator between semiconductor and the metal gate contact. Such a thin film is made by  either thermal evaporation, or simply spin coating. In a TFT device, there is no carrier movement between the source and drain. After applying a positive charge, accumulation of electrons on the interface cause bending of the semiconductor and ultimately lowers the conduction band with regards to the Fermi-level of the semiconductor. Finally, a highly conductive channel is formed at the interface. Features. Conductive polymers are lighter, more flexible, and less expensive than inorganic conductors. This makes them a desirable alternative in many applications. It also creates the possibility of new applications that would be impossible using copper or silicon . Organic electronics not only includes organic semiconductors, but also organic dielectrics, conductors and light emitters. New applications include smart windows and electronic paper. Conductive polymers are expected to play an important role in the emerging science of molecular computers.